User Rating: / 0
PoorBest
Written by Chris Denney
Tuesday, 29 January 2013 18:28

### Considering the two schools of thought for the angle at which the solder nozzle leaves a header strip.

This is the first in a series of columns discussing tips and tricks for using a selective soldering machine.

When soldering a double row header, or similar part, the solder can easily bridge at the end where the solder nozzle comes off. I don’t know the technical term for this but I call it the “drag off.” There are multiple arguments for the way you can drag off the end of the double row header. The most common recommendation is to drag off at a 45⁰ angle.

I don’t necessarily agree with this. I found greater success dragging off parallel with the double row (in other words, straight). The key here is the speed you drag off at. The slower the better. (You can go too slowly though, so be careful. If you go too slowly, you’ll melt the header you’re soldering.) More important, you need to use that same speed across the entire header. The trouble is, when the nozzle changes speeds or angles, it stutters, but not much. It’s almost imperceptible, but if you look closely, you’ll see it. I don’t know that this is necessarily what causes the bridging, but I suspect it is. So what we do more often than not is drag straight off the double row headers at 0.200" per second.

Now, after explaining all of that, I must point out that sometimes it is still necessary to drag off at a 45⁰ angle. Take a look at Figure 1. You’ll see two double row headers. The one on the left we drag off at a 45⁰ angle. The one on the right we drag off straight.

You’ll notice that on the double row header where we drag off at a 45⁰ angle, the pivot point is right at the last two pins, while still barely touching the previous two pins. What’s happening here, as best I can understand, is that we change all the surface tension of the solder wave. We now have four pins all tugging at the solder as it’s dragging off. This causes the solder to want to adhere just to the pins and not to fall back onto itself. That said, I’ve still had better success dragging off at a straight angle, without “stutter stepping” on the last four pins.

To sum up, try dragging off at a straight angle, making sure to go slowly over the whole double row header. We find 0.200" per second works best. If you get inconsistent results with that technique, try dragging off at a 45⁰ angle, making sure your pivot point is adhering to the last four pins to use them as tension against the solder bridging itself.

If you have any questions, feel free to contact me at This e-mail address is being protected from spambots. You need JavaScript enabled to view it .

Chris Denney is chief technology officer at Worthington Assembly (worthingtonassembly.com) This e-mail address is being protected from spambots. You need JavaScript enabled to view it .

Last Updated on Tuesday, 16 April 2013 13:59

### Columns

 M&A is Here to Stay
 There’s been a flurry of EMS acquisition activity of late, with Natel’s acquisition of EPIC Technologies and Benchmark’s pickup of Suntron and CTS among the larger deals. Read more...

 What Does New CEO for Microsoft Mean for Hardware?
 In the end, Microsoft couldn't pull the trigger. In Seattle, outside just wasn't "in." The world's largest software developer today named Satya Nadella, head of the the company’s Server and Tools unit, as its new chief executive. The 46-year-old Nadella becomes just the third person to lead Microsoft, one of the most successful and wealthiest companies ever. Read more...

### Features

 A Systems-Level Approach to Product Development
 Is there a way to more tightly integrate materials and process development so as to accelerate the pace of innovation? Read more...

 Reducing Stencil Wipe Frequency
 A new study of nanocoatings allows users to visualize solder paste flow under the stencil. Read more...

## Language

### Products

Getech Releases GLRS Laser Singulater
GLRS laser singulation system is configurable with a near IR laser (1032nm) for use with metal-core substrates or a green laser (532 nm) for use with ultra-thin and flexible substrates. Inert gas...